Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements


 William Hudson
 1 years ago
 Views:
Transcription
1 Acta Mech. Sin. (2016) 32(2): DOI /s RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1 H. Puga 1 J. Meireles 1 Received: 28 September 2014 / Revised: 15 March 2015 / Accepted: 16 April 2015 / Published online: 17 November 2015 The Chinese Society of Theoretical and Applied Mechanics; Institute of Mechanics, Chinese Academy of Sciences and SpringerVerlag Berlin Heidelberg 2015 Abstract Materials with a negative Poisson s ratio (PR) are called auxetics; they are characterized by expansion/ contraction when tensioned/compressed. Given this counterintuitive behavior, they present very particular characteristics and mechanical behavior. Geometrical models have been developed to justify and artificially reproduce such materials auxetic behavior. The focus of this study is the exploration of a reentrant model by analyzing the variation in the PR of reentrant structures as a function of geometrical and base material parameters. It is shown that, even in the presence of protruding ribs, there may not be auxetic behavior, and this depends on the geometry of each reentrant structure. Values determined for these parameters can be helpful as approximate reference data in the design and fabrication of auxetic lattices using reentrant geometries. Keywords Auxetic Poisson s ratio Reentrant Finite element analysis Elasticity 1 Introduction Poisson s ratio (PR) is a dimensionless constant that describes the negative ratio of lateral strain to the longitudinal strain on a tensioned body. As common sense dictates, the cross section of a body becomes larger/thinner in compression/tension, so the value of this constant is assumed to B V. H. Carneiro 1 Department of Mechanical Engineering, University of Minho, Campus de Azurem, Guimarães, Portugal be positive [1]. However, considering the classical theory of elasticity, it is possible to observe that this constant may assume values from 1 to 0.5 in threedimensional isotropic bodies [2] and between 1 and 1 in twodimensional isotropic materials [3]. For anisotropic materials, this constant depends on the stretch and transverse direction and may assume values other than the previously established ones [4]. Materials that present a generalized negative PR are called auxetics [5]. Anisotropic materials that reveal only negative values of PR along certain directions are called partial auxetics [6]. Owing to the negative value of this constant, these materials are endowed with very particular characteristics and peculiar mechanical behavior [7]. Some examples are their superior resistance to indentation, shear and fracture, enhanced acoustic absorption, synclastic behavior, variable permeability, and shape memory characteristics [1]. Some geometric models have been developed to justify this unusual behavior; among them, the most common are the reentrant, chiral, and semirigid rotating models (e.g., Ref. [7]). It is commonly accepted that these models always demonstrate auxetic behavior; however, this may not always be true [8]. This study analyzes whether the presence of protruding ribs in a reentrant structure is enough to produce auxetic behavior in reentrant structures. The experimental study of such models, by considering how they are made and conducting experiments on them, is an elaborate and complex task. It is convenient to resort to finiteelement (FE) analysis to analyze them (e.g., Refs. [3,9]). The use of such techniques is a very efficient and a quick way to manipulate and determine the behavior of different reentrant models [10]. Consequently, these routines make it possible to determine the parameters that influence the auxetic behavior of these structures.
2 296 V. H. Carneiro et al. Fig. 1 a Individual cell in reentrant lattice. b Base analyzed reentrant structure The objective of the present article is the study of the parameters that influence the auxetic behavior of reentrant structures using FE analysis, considering the variation in the geometrical and base material characteristics. This study may lead to the tailoring of these structures and permit the application of lattices (periodic structures composed by struts [11]) with a projected PR in practical applications. Additionally, the relative densities of the simulated reentrant structures will be determined considering different geometries so as to generate values of critical relative density in the transition between auxetic and nonauxetic behavior. 2 Methodology The fundamental objective of this study is the definition of the variables that determine the presence of auxetic behavior in a reentrant twodimensional structure (Fig. 1a). To this end, numerical simulations (using FE analysis) were conducted to model a base reentrant structure (Fig. 1b), varying some structural characteristics and applying a quasistatic tensile load (F1 ) on the XXaxis (the value of the load assured that the structures never experienced plastic deformation). This method was adopted so the inertial terms would be negligible. The resultant deformations made it possible to determine the PR of the structure and, consequently, the presence/absence of auxetic behavior. 2.1 Structural characteristics: geometry and base material properties The modified characteristics were divided into two main categories: the geometrical and the base material parameters. In the first category, the variation consisted in changing the length (a), width (c), and initial angle (β) of the ribs of the initial reentrant structures (Fig. 1, Table 1). The base material of the structure was defined as linear elastic and isotropic. This implies that its elastic behavior can be defined by only two of the four basic isotropic elastic Table 1 Initial structural and modified structural characteristics Parameter Initial E (Young s modulus: base material) 200 ν (Poisson s ratio: base material) 0.3 a (Length) 40 c (Width) 6 β (Angle) 45 F (Load) 20 Modified Units GPa mm mm ( ) N constants [12]. In this approach, the selected elastic constants were the Young s modulus and the PR. These constants completely characterize the elastic behavior of the structures. Given that the reentrant structures are represented in two dimensions, they were simplified in the simulations using plane stress conditions. The other elastic constants, the bulk (K ) and shear (G) moduli, can be determined considering the adopted simplification by Eqs. (1) and (2) [13]: E, 2(1 ν) E G=. 2(1 + ν) K = (1) (2) 2.2 Structure simulation: finiteelement analysis characteristics To determine the PR of the structures, whose parameters were varied, a simulation was conducted using FE analysis. The type of simulation used was a linear elastic plane stress model, considering that the base material is isotropic. Thus, the deformation behavior of the body was regulated by Hooke s law (Eq. (3)): σi j = D εi j. (3) The stress (σ ) in the structure is generated by the quasistatic unitary force (F1 : Fig. 1a), applied on the XXaxis to
3 Analysis of the geometrical dependence of auxetic behavior 297 Table 2 Mesh characteristics Mesh settings Value Finally, the PR of the analyzed structures can be simply determined using Eq. (8): Maximum element size Minimum element size 0. Maximum element growth rate Resolution of curvature Resolution of narrow regions the structure (initially in a free body). In isotropic materials, the twodimensional stiffness matrix D is defined by Eq. (4): 1 ν 0 E D = (1 ν 2 ν 1 0. (4) ) ν This relation implies that there are deformations imposed on the structure. The observed deformation may also be generally expressed on a given axis, in the form of strain, by Eq. (5): ε = 1 2 ( u + u T). (5) Using FE analysis, the previously defined equations may be used to determine the strain of the nodes that compose the mesh in which the analyzed body is subdivided. The numerical computation was performed using COMSOL Multiphysics. The mesh created by that software was built using the preset parameter values in the Extra fine mesh function (see Table 2 for settings). To generate the desired results, the software used the MUltifrontal Massively Parallel sparse direct Solver (MUMPS solver). 2.3 Determination of Poisson s ratio of reentrant structures To determine the PR of each analyzed structure and the presence/absence of auxetic behavior, the strain values were monitored in two nodes (Fig. 1). Node 1 is placed on the axis of the imposed tensile load and will only deform in that direction (XXaxis). Node 2 was placed such that it deforms only along the YYaxis, following the expansion/contraction of the protruding ribs. Thus, by the definition and monitoring of these two nodes, it is possible to determine the longitudinal (XXaxis) and transverse (YYaxis) strains of each analyzed structure using Eqs. (6) and (7): ( ) u ε (xx, Structure) = 2 x, node 1, (6) ( ) v ε (yy, Structure) = 2 y, node 2. (7) ν Structure = ε (xx, Structure) ε (yy, Structure). (8) 3 Results and discussion The role of the rib width was verified (Fig. 2) in the deformation mechanism of a reentrant structure. Its value was varied and numerical simulations were conducted, with the parameters mentioned previously, to calculate the PR of the individual reentrant structure. It can be observed in Fig. 2 that the rib width has a direct influence on the value of the PR of a reentrant structure. As the rib width increases, so does the general value of the PR in a reentrant structure. The increase in the PR with the rib width can be interpreted in the following way. When there is a small rib width, there are significant deformations even for small loads. The structure itself is not very rigid and behaves like a spring, forcing a significant vertical expansion. On the other hand, increasing the rib width will generate a stiffer structure. This change will eventually culminate in the loss of auxetic behavior, as the internal space and, consequently, the protruding ribs tend to be eliminated by the increase in the rib width. The role of the rib length (Fig. 3) was analyzed. Its value was varied and numerical simulations were conducted to determine the resulting structure s PR. Analyzing Fig. 3, it can be observed that the rib length is a key parameter in the determination of the PR of a reentrant structure. It is shown that when the rib length increases, the actual PR of the reentrant structure decreases. This can be justified by the spring behavior of the reentrant struc Fig. 2 Variation of structure s PR by changing the rib width (a = 40 mm, β= 45, E = 200 GPa, ν= 0.3)
4 298 V. H. Carneiro et al. Fig. 3 Variation of structure s PR by changing the rib length (c = 6mm,β= 45, E = 200 GPa, ν= 0.3) Fig. 5 Variation of structure s PR by changing the rib angle (a = 40 mm, c = 6mm, E = 200 GPa, ν= 0.3) Fig. 4 Variation of structure s PR by keeping the rib s AR at 5 (β = 45, E = 200 GPa, ν= 0.3) ture. When the rib length is increased, the general structure stiffness decreases. This fact leads to significant deformations and to the vertical expansion that characterizes auxetic behavior. Observing the previous results in Fig. 3, it can be concluded that the auxetic behavior of a reentrant structure depends on the rib length and width. These values are mainly related to the length and width of the ribs, which will determine the stiffness of the structure. Therefore, simulations were conducted to determine the dependence of the PR of the structure on the aspect ratio (AR) between the length and the width of a structure s ribs (Fig. 4). The value of the rib length was varied, but the proportion of the AR was kept constant at a value of 5. According to Fig. 4, it can be observed that when the AR is kept constant, the PR of the structure remains constant as well. Another analyzed parameter was the initial angle between ribs, as shown in Fig. 5. Numerical simulations were conducted with different values of the initial angles, and the importance of a reentrant structure in the deformation mechanism was verified. Fig. 6 Variation of structure s PR by changing the base material PR and Young s modulus (a = 40 mm, c = 6mm,β= 45 ) Observing Fig. 5, it can be concluded that the PR of a reentrant structure is influenced by the initial angle between ribs. When the angle decreases, there is a similar decrease in the value of the structure s PR. However, for extremely low values of rib angles, the PR increases. A decrease in the rib angle generates a decrease in the free interior structural space. In extreme cases, this space ceases to exist, eliminating the reentrant structure. Proceeding to the base material parameters, the PR and Young s modulus of the base material were analyzed to determine their influence on the deformation behavior of a reentrant structure. Geometrical equivalent base structures were simulated based on Fig. 1b, varying the PR and the Young s modulus of the base material. The results are presented in Fig. 6. It is shown the PR of the reentrant structure remains stable when the PR of the base material is changed. Note that the
5 Analysis of the geometrical dependence of auxetic behavior 299 Table 3 PR of reentrant structure for different ARs and rib angles (E = 200 GPa, ν = 0.3) Fig. 7 Variation of structure s PR using the rib angle for different ARs two do not predominate when describing the deformation mechanism of a reentrant structure. As may be observed, the value of the PR of the reentrant structure remained constant when the Young s modulus of the base material was changed. In this way, it is shown that the PR of a reentrant structure is independent of the value of the Young s modulus of the base material. Having isolated all the fundamental parameters that describe the deformation mechanism of a reentrant structure, we can establish that the auxetic behavior will mainly depend on the interaction of the length, width, and angle of the ribs. Because the PR of a reentrant structure remains constant for the same rib AR, these two parameters can be analyzed using only one ratio. With the facts presented, and carrying out numerical simulations, the obtained information was used to create Table 3. Looking at Table 3, it can be observed that there is a dependence between the auxetic behavior, low values of rib angles, and high values of AR. According to the executed simulations and the resulting data, it was possible to elaborate Fig. 7. Boundaries relating the structure s AR and initial rib angle were established that might predict whether a reentrant structure will demonstrate auxetic behavior and show the specific values of the PR. In terms of relative density, it can be observed in Fig. 8 that the values of AR and initial rib angle generate a parabola shape function. When the values of the initial rib angle are extreme (either high or low), the values of the relative density tend to decrease. However, only low values of AR Fig. 8 Relative density of reentrant structures as a function of rib angle and AR tend to increase this effect. It can also be observed that each AR that demonstrates auxetic behavior has a specific value of the critical relative density where the transition between auxetic/nonauxetic behavior takes place. Considering the aforementioned plots, it is suggested that the value of the critical density is lower in the presence of a low AR. In contrast, for low initial rib angles the value of the critical relative density tends to increase. Given that a low AR implies thinner and longer ribs, the overall relative density tends to decrease. However, in the case of the initial rib angle, the structure tends to fold on itself, closing the opening in its interior and generating higher relative density values. 4 Conclusions Considering the results of the executed numerical simulations, it was shown that a reentrant structure, even in the presence of protruding ribs, may not always demonstrate auxetic behavior. This study isolated the length, width (mainly the AR), and initial angle of the structure s ribs
6 300 V. H. Carneiro et al. as the predominant factors that determine auxetic behavior. It was also observed that the characteristics of the base material that composes the structures, such as the constants that describe elastic deformation, may have less influence on the auxetic behavior of a reentrant structure. Limits to the values of length, width, and angles of the ribs were defined to obtain and tailor a predetermined value of the PR of these structures. This allows for the development of structures with a defined PR, even in the project phase, using the same base geometry. According to this formulation, the obtained value of PR is directly related to the unitary reentrant structure. In the case of their application in a lattice, the obtained value of the macroscopic PR may vary slightly, given that the ribs that connect the individual reentrant structures are also elastic. However, as the present study suggests, the main deformation mechanism used to induce auxetic behavior is the bending of the protruding ribs, and this implies a low AR of the ribs. The elastic deformation of the ribs that connect each individual reentrant structure (the ones that do not protrude) is mainly the result of tensile and compressive forces. This last forces, in connection with macroscopic deformation, are negligible compared to the overall reentrant structure expansion. Additionally, the value of the critical relative density at which the transition between auxetic and nonauxetic behavior occurs was determined. It was shown that this value tends to increase for lower initial rib angles. However, in the presence of a low AR, the value of the critical relative densities tends also to decrease. The generated values of the relative density may also be used in a project phase as an input on weight and overall structural performance when projecting an auxetic lattice. References 1. Carneiro, V.H., Puga, H., Meireles, J.: Auxetic materials a review. Mater. Sci. Pol. 31, (2013) 2. Mott, P.H., Roland, C.M.: Limits to Poisson s ratio in isotropic materials general results for arbitrary deformation. Phys. Scr. 87, (2013) 3. Strek, T., Maruszewski, B., Narijczyk, J.W., et al.: Finite element analysis of plate deformation. J. Noncryst. Solids 354, (2008) 4. Norris, A.N.: Extreme values of Poisson s ratio and other engineering moduli in anisotropic materials. J. Mech. Mater. Struct. 1, (2006) 5. Dirrenberger, J., Forest, S., Jeulin, D.: Elastoplasticity of auxetic materials. Comput. Mater. Sci. 64, (2012) 6. Brańka, A.C., Heyes, D.M.: Maćkowiak, Sz, et al.:cubic materials in different auxetic regions linking microscopic to macroscopic formulations. Phys. Status Solidi B 249, (2012) 7. Critchley, R., Corni, I., Wharton, J.A., et al.: A review of the manufacture, mechanical properties and potential applications of auxetic foams. Phys. Status Solidi B 250, (2013) 8. Liu, Y., Hu, H.: A review in auxetic structures and polymeric materials. Sci. Res. Essays 5, (2010) 9. Bückmann, T., Schittny, R., Thiel, M., et al.: On threedimensional dilational elastic metamaterials. N. J. Phys. 16, (2014) 10. Pozniak, A.A., Smardzewski, J., Wojciechowski, K.W.: Computer simulations of auxetic foams in twodimensions. Smart Mater. Struct. 22, (2013) 11. Fan, H.L., Zeng, T., Fang, D.N., et al.: Mechanics of advanced fiber reinforced lattice composites. Acta Mech. Sin. 26, (2010) 12. Du, D.X., Zheng, Q.S., Gao, Y.X.: Consistency between independence theorems and generalized selfconsistent method. Acta Mech. Sin. 13, (1997) 13. Jasiuk, I., Chen, J., Thorpe, M.F.: Elastic moduli of two dimensional materials with polygonal and elliptical holes. Appl. Mech. Rev. 47, (1994)
Threedimensional stiff cellular structures with negative Poisson's ratio
! Threedimensional stiff cellular structures with negative Poisson's ratio Dong Li a, Jie Ma a, Liang Dong b and Roderic S. Lakes c a College of Sciences, Northeastern University, Shenyang 110819, PR
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationPoisson s ratio of rectangular antichiral lattices with disorder
Poisson s ratio of rectangular antichiral lattices with disorder Artur A. Poźniak 1 Krzysztof W. Wojciechowski 2 1 Institute of Physics, Poznań Universty of Technology, ul. Nieszawska 13A, 60695 Poznań,
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationForced Response of Plate with Viscoelastic Auxetic Dampers
Vibrations in Physical Systems 2018, 29, 2018003 (1 of 9) Abstract Forced Response of Plate with Viscoelastic Auxetic Dampers Tomasz STREK Poznan University of Technology, Institute of Applied Mechanics
More informationPlanar auxeticity from various inclusions
Planar auxeticity from various inclusions Artur A. Poźniak 1 Krzysztof W. Wojciechowski 2 Joseph N. Grima 3 Luke Mizzi 4 1 Institute of Physics, Poznań Universty of Technology, Piotrowo 3, 6695 Poznań
More information20. Rheology & Linear Elasticity
I Main Topics A Rheology: Macroscopic deformation behavior B Linear elasticity for homogeneous isotropic materials 10/29/18 GG303 1 Viscous (fluid) Behavior http://manoa.hawaii.edu/graduate/content/slidelava
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationANOMALOUS DEFORMATION OF CONSTRAINED AUXETIC SQUARE
Anomalous Rev.Adv.Mater.Sci. deformation 23(2010) of constrained 169174 auxetic square 169 ANOMALOUS DEFORMATION OF CONSTRAINED AUXETIC SQUARE Artur A. PoŸniak 1, Henryk Kamiñski 2, Przemys³aw Kêdziora
More informationMechanical Properties
Mechanical Properties Elastic deformation Plastic deformation Fracture I. Elastic Deformation S s u s y e u e T I II III e For a typical ductile metal: I. Elastic deformation II. Stable plastic deformation
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationExtreme Cosserat elastic cube structure with large magnitude of negative Poisson s ratio
Extreme Cosserat elastic cube structure with large magnitude of negative Poisson s ratio Carlos Andrade Chan Soo Ha +,androderics.lakes? December 7, 2018 Department of Engineering Physics, Department of
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationChapter 2: Elasticity
OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More information548 Advances of Computational Mechanics in Australia
Applied Mechanics and Materials Online: 20160725 ISSN: 16627482, Vol. 846, pp 547552 doi:10.4028/www.scientific.net/amm.846.547 2016 Trans Tech Publications, Switzerland Geometric bounds for bucklinginduced
More informationChapter Two: Mechanical Properties of materials
Chapter Two: Mechanical Properties of materials Time : 16 Hours An important consideration in the choice of a material is the way it behave when subjected to force. The mechanical properties of a material
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationTwodimensional Phosphorus Carbide as Promising Anode Materials for Lithiumion Batteries
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A. This journal is The Royal Society of Chemistry 2018 Supplementary Material for Twodimensional Phosphorus Carbide as Promising
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationHomogenization on MultiMaterials Elements: Application to Printed Circuit Boards and Warpage Analysis
Homogenization on MultiMaterials Elements: Application to Printed Circuit Boards and Warpage Analysis Manuel Araújo 1,a, J. L. Alves 1, Paulo Silva 1 and Pedro Delgado 2 1 MEMS, University of Minho, Dep.
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationComputer simulation of the Poisson's ratio of soft polydisperse discs at zero temperature
Computer simulation of the Poisson's ratio of soft polydisperse discs at zero temperature JAKUB NAROJCZYK KRZYSZTOF W. WOJCIECHOWSKI Institute of Molecular Physics Polish Academy of Sciences ul. M. Smoluchowskiego
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationElasticity in two dimensions 1
Elasticity in two dimensions 1 Elasticity in two dimensions Chapters 3 and 4 of Mechanics of the Cell, as well as its Appendix D, contain selected results for the elastic behavior of materials in two and
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationINFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK BETWEEN THE TWO LAYERS
Djoković, J. M., et.al.: Influence of Temperature on Behavior of the Interfacial THERMAL SCIENCE: Year 010, Vol. 14, Suppl., pp. S59S68 S59 INFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationMacroscopic theory Rock as 'elastic continuum'
Elasticity and Seismic Waves Macroscopic theory Rock as 'elastic continuum' Elastic body is deformed in response to stress Two types of deformation: Change in volume and shape Equations of motion Wave
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationInternational Journal of Scientific & Engineering Research Volume 8, Issue 12, December2017 ISSN
362 Study of the Effects of Random Inclusions in Composite Construction with Isotropic Negative Poisson s Ratio [Kundan Singh Deshwal1, a and Dr. Satyendra Singh2, b] 1 Assistant Professor, Department
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationModelling and numerical simulation of the wrinkling evolution for thermomechanical loading cases
Modelling and numerical simulation of the wrinkling evolution for thermomechanical loading cases Georg Haasemann Conrad Kloß 1 AIMCAL Conference 2016 MOTIVATION Wrinkles in web handling system Loss of
More informationComputational Modelling of Vibrations Transmission Loss of Auxetic Lattice Structure
Vibrations in Physical Systems Vol. 27 (2016) Abstract Computational Modelling of Vibrations Transmission Loss of Auxetic Lattice Structure Eligiusz IDCZAK Institute of Applied Mechanics, Poznan University
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationMacroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs
Macroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs JingZhong Xie 1 Abstract: The macroscopic Poisson ratio and elastic moduli of the castinplace hollowcore slab are researched
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More information3D Finite Element Analysis of Instrumented Indentation of Transversely Isotropic Materials
3D Finite Element Analysis of Instrumented Indentation of Transversely Isotropic Materials Abstract: Talapady S. Bhat and T. A. Venkatesh Department of Material Science and Engineering Stony Brook University,
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationUltimate shear strength of FPSO stiffened panels after supply vessel collision
Ultimate shear strength of FPSO stiffened panels after supply vessel collision Nicolau Antonio dos Santos Rizzo PETROBRAS Rio de Janeiro Brazil Marcelo Caire SINTEF do Brasil Rio de Janeiro Brazil Carlos
More informationIDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationREPORT TO DFLEX LTD APRIL 2009 REPORT. (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009)
REPORT (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009) Finite Element Modelling of Rigidity of Fishing Rods with Various Crosssections Report to DFlex Ltd by Z Guan Department of Engineering,
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationMASONRY MICROMODELLING ADOPTING A DISCONTINUOUS FRAMEWORK
MASONRY MICROMODELLING ADOPTING A DISCONTINUOUS FRAMEWORK J. PinaHenriques and Paulo B. Lourenço School of Engineering, University of Minho, Guimarães, Portugal Abstract Several continuous and discontinuous
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationFinite element analysis of FRP pipelines dynamic stability
Boundary Elements and Other esh Reduction ethods XXXVIII 39 Finite element analysis of FRP pipelines dynamic stability D. G. Pavlou & A. I. Nergaard Department of echanical and Structural Engineering and
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationNumerical evaluation of effective material properties of randomly distributed short cylindrical fibre composites
Computational Materials Science 39 (2007) 198 204 www.elsevier.com/locate/commatsci Numerical evaluation of effective material properties of randomly distributed short cylindrical fibre composites S. Kari
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationDetermination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test
Rock Mech Rock Eng DOI 10.1007/s0060301405869 TECHNICAL NOTE Determination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test Xiangtao Xu Runqiu Huang Hua
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationResearcher s name: Stanislav Stoykov Scientific advisor: Prof. Svetozar Margenov /host professor/ Working period: 16 October March 2014
Advanced Computing for Innovation RESEARCH REPORT for work performed under longterm employment /experienced researchers with less than 10 years of scientific experience incl. postdocs/ Researcher s name:
More informationApplication of nanoindentation technique to extract properties of thin films through experimental and numerical analysis
Materials SciencePoland, Vol. 28, No. 3, 2010 Application of nanoindentation technique to extract properties of thin films through experimental and numerical analysis A. WYMYSŁOWSKI 1*, Ł. DOWHAŃ 1, O.
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationOptimum Height of Plate Stiffener under Pressure Effect
The st Regional Conference of Eng. Sci. NUCEJ Spatial ISSUE vol., No.3, 8 pp 459468 Optimum Height of Plate Stiffener under Pressure Effect Mazin Victor Yousif M.Sc Production Engineering University of
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationOn the geometric and material nonlinearity effects of polymeric thin plates or films on structural performance.
On the geometric and material nonlinearity effects of polymeric thin plates or films on structural performance. Kiran V, Asutosh P and Raj C Thiagarajan ATOA Scientific Technologies Pvt Ltd ATOA Scientific
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationWeight and contact forces: Young's modulus, Hooke's law and material properties
Weight and contact forces: Young's modulus, Hooke's law and material properties Many objects deform according to Hooke's law; many materials behave elastically and have a Young's modulus. In this section,
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationCHAPTER 5. Beam Theory
CHPTER 5. Beam Theory SangJoon Shin School of Mechanical and erospace Engineering Seoul National University ctive eroelasticity and Rotorcraft Lab. 5. The EulerBernoulli assumptions One of its dimensions
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationSTRESS, STRAIN AND DEFORMATION OF SOLIDS
VELAMMAL COLLEGE OF ENGINEERING AND TECHNOLOGY, MADURAI 625009 DEPARTMENT OF CIVIL ENGINEERING CE8301 STRENGTH OF MATERIALS I 
More informationNDT&E Methods: UT. VJ Technologies CAVITY INSPECTION. Nondestructive Testing & Evaluation TPU Lecture Course 2015/16.
CAVITY INSPECTION NDT&E Methods: UT VJ Technologies NDT&E Methods: UT 6. NDT&E: Introduction to Methods 6.1. Ultrasonic Testing: Basics of ElastoDynamics 6.2. Principles of Measurement 6.3. The PulseEcho
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationMODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES
MODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES P.J.Hine*, C.D.Price*, B.Whiteside $, A.M.Cunha # and I.M.Ward* *  IRC in Polymer Science and Technology, University
More informationMODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD
MODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD Andrzej Skrzat, Rzeszow University of Technology, Powst. Warszawy 8, Rzeszow, Poland Abstract: Userdefined material models which can be used
More informationConstitutive model for quasistatic deformation of metallic sandwich cores
INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng 2004; 61:2205 2238 Published online 18 October 2004 in Wiley InterScience (www.interscience.wiley.com). DOI: 10.1002/nme.1142
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationRock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth
Rock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth References: Turcotte and Schubert, Geodynamics, Sections 2.1,2.4, 2.7, 3.13.8, 6.1, 6.2, 6.8, 7.17.4. Jaeger and Cook, Fundamentals of
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More information